Structural evaluation of sugar cane bagasse steam pretreated in the presence of CO2 and SO2
- Roberta Cristina Novaes Reis Corrales1,
- Fabiana Magalhães Teixeira Mendes1,
- Clarissa Cruz Perrone1,
- Celso Sant’Anna2, 3,
- Wanderley de Souza2, 3,
- Yuri Abud2,
- Elba Pinto da Silva Bon4 and
- Viridiana Ferreira-Leitão1, 4Email author
© Corrales et al.; licensee BioMed Central Ltd. 2012
Received: 13 February 2012
Accepted: 22 May 2012
Published: 22 May 2012
Previous studies on the use of SO2 and CO2 as impregnating agent for sugar cane bagasse steam treatment showed comparative and promising results concerning the cellulose enzymatic hydrolysis and the low formation of the inhibitors furfural and hydroxymethylfurfural for the use of CO2 at 205°C/15 min or SO2 at 190°C/5 min. In the present study sugar cane bagasse materials pretreated as aforementioned were analyzed by scanning and transmission electron microscopy (SEM and TEM), X-Ray Diffraction (XRD) and Infrared (FTIR spectroscopy) aiming a better understanding of the structural and chemical changes undergone by the pretreated materials.
SEM and TEM data showed that the structural modifications undergone by the pretreatment with CO2 were less pronounced in comparison to that using SO2, which can be directly related to the combined severity of each pretreatment. According to XRD data, untreated bagasse showed, as expected, a lower crystallinity index (CI = 48.0%) when compared to pretreated samples with SO2 (CI = 65.5%) or CO2 (CI = 56.4%), due to the hemicellulose removal of 68.3% and 40.5%, respectively. FTIR spectroscopy supported SEM, TEM and XRD results, revealing a more extensive action of SO2.
The SEM, TEM, XRD and FTIR spectroscopy techniques used in this work contributed to structural and chemical analysis of the untreated and pretreated bagasse. The images from SEM and TEM can be related to the severity of SO2 pretreatment, which is almost twice higher. The crystallinity index values obtained from XRD showed that pretreated materials have higher values when compared with untreated material, due to the partial removal of hemicellulose after pretreatment. FTIR spectroscopy supported SEM, TEM and XRD results. CO2 can actually be used as impregnating agent for steam pretreatment, although the present study confirmed a more extensive action of SO2.
KeywordsSugar cane bagasse CO2 and SO2 steam pretreatment SEM and TEM microscopy XRD and FTIR spectroscopy
Fourier transform infrared spectroscopy
Scanning electron microscopy
Transmission electron microscopy
X-Ray diffraction spectroscopy
There is a growing urgency to develop novel bio-based products and other innovative technologies that can overcome the widespread dependence on fossil fuels . Unlike gasoline, ethanol is a renewable energy source produced through fermentation of sugar. In Brazil, ethanol is produced largely from sugar cane juice, known as first generation (1G) ethanol. The residual lignocellulosic biomass from the 1G ethanol industry (sugar cane bagasse and leaves) is, presently, for a collection of reasons, the most promising resource for the production of lignocellulosic (2G) ethanol . However, although the sugar-ethanol industry generates bagasse in large quantities during the process of extraction of the sugar cane juice it is mostly used for co-generation, accounting for approximately 3% of the electricity available in Brazil .
Lignocellulosic biomass is mainly composed of cellulose, hemicellulose and lignin. The predominant component of lignocellulosic biomass is cellulose, a linear β (1,4)-linked chain of glucose molecules. It is non-toxic, renewable, biodegradable, modifiable and has great potential as an excellent industrial material [4, 5]. The elementary fibrils are composed of crystalline and amorphous regions. Hemicelluloses are made up of C5 and C6 sugar, such as xylose, arabinose, galactose, glucose and mannose. Lignin accounts for about one fourth of the lignocellulosic biomass and is the third most abundant biopolymer only after cellulose and hemicellulose.
According to Fengel and Wegener , four elementary fibrils of cellulose are held together by a monolayer of hemicellulose, which generate 25 nm wide thread-like structures that are enclosed in a matrix of hemicellulose and lignin (associated with each other through physical interactions and covalent bonds).
The main steps for ethanol production from lignocellulosic biomass are pretreatment, hydrolysis, fermentation and distillation/purification. The pretreatment should enhance the fiber accessibility and consequently facilitate the subsequent steps of enzymatic hydrolysis and fermentation .
The raw material pretreatment step could represent up to 20% of the total costs of cellulosic ethanol production . According to Galbe and Zacchi , an effective pretreatment should (a) improve cellulose digestibility; (b) produce low concentrations of degradation products derived from sugars and lignin; and (c) have a low energy demand.
Previous studies on steam pretreatment of bagasse employed CO2 as impregnating agent to replace the traditionally used SO2. The use of CO2 was previously investigated in order to explore some advantages of this gas over SO2, such as high availability in the first-generation ethanol plants, low toxicity, low corrosivity and low occupational risk [10, 11]. Although the use of CO2 provided equivalent results in comparison to those obtained when SO2 was used as impregnating agent, higher temperatures or longer times were necessary. Comparative results concerning glucose release and inhibitors formation (furfural and hydroxymethylfurfural – HMF) from steam pretreated bagasse were obtained under the conditions: 205°C/15 min using CO2 or 190°C/5 min using SO2. As previously reported by authors , the use of SO2 resulted in 79.7% of glucose after enzymatic hydrolysis and provided the formation of 0.80 g/100g of furfural and 0.18 g/100g of HMF (dry bagasse). When CO2 was employed, the yield of glucose reached 86.6% and the values for furfural (0.9 g/100g) and HMF (0.2 g/100g) were very similar to those reported for SO2.
FTIR spectroscopy and electron microscopy have been used for the analysis of structural and morphological modifications in the biomass after pretreatment [12–14]. The present work evaluated structural and chemical changes of SO2 and CO2 steam pretreated sugar cane bagasse in comparison to the untreated material using electron microscopy, X-ray diffraction (XRD) and infrared spectroscopy (FTIR).
Results and discussion
Scanning electron microscopy (SEM) and transmission electron microcopy (TEM)
Untreated bagasse sample (Figure 1A, B, C) presents a rigid and compact morphology, while the ones submitted to pretreatment with SO2 (Figure 1D, E, F) or CO2 (Figure 1G, H, I) exhibited a more disorganized morphology, with greater exposure of the fibers.
After pretreatment, the most exposed cell wall structure allows for a greater accessibility to hydrolytic enzymes, which facilitates the hydrolysis of lignocellulosic biomass.
Data from SEM and TEM showed that both pretreatments were effective with respect to structural changes, increasing the surface exposure of the bagasse samples. However, the morphology of CO2 pretreated material is more preserved than that of the SO2 material. This result can be directly related to the higher combined severity for the pretreatment using SO2 (1.7), when compared to combined severity of the pretreatment with CO2 (0.9) as impregnating agent. It is important to emphasize that the combined severity factor  takes into account besides time and temperature of the steam pretreatment, the acidity generated in the reaction media by the formation of sulfuric and carbonic acid and the release of organic acids, such as acetic acid from the raw material, as indicated by the pH drop after pretreatment (pH 1.7 (SO2); pH 3.8 (CO2)) .
X-ray diffraction (XRD)
Figure 3 shows diffractograms of untreated bagasse (A) and sugar cane bagasse pretreated with SO2 (B) or CO2 (C). As can be observed, all samples exhibit typical cellulose diffraction peaks, where the highest peak corresponds to the 002 crystallographic planes. The crystallinity index was calculated according to Equation 1 (Methods session). The untreated sugar cane bagasse showed a lower crystallinity (CI = 48.0%) when compared to samples pretreated with SO2 (CI = 65.5%) and CO2 (CI = 56.4%). Many studies indicate that there is an increase in the value of this index when the biomass is subjected to pretreatment by steam explosion . The phenomenon is due mainly to the removal of a certain amount of lignin and hemicellulose (amorphous substances) and not necessarily due to changes in the crystalline structure of the biomass.
As expected the crystallinity index for the bagasse pretreated with SO2 (65.5%) was higher than that of CO2 pretreated bagasse (56.4%). Indeed, it was observed a more effective removal of hemicellulose to the liquid fraction (63.8%: 7.0% xylose as oligomers and 56.8% of monomeric xylose) using the SO2 steam pretreatment than that using CO2 that showed 40.5% hemicellulose removal : (21.5%) of xylose in oligomeric form and 19.0% in monomeric form) . In this work, the increase of the crystallinity index in the pretreated samples is explained by the partial removal of hemicellulose fraction. The amount of glucose released from cellulose (amorphous region) was not relevant in the pretreatment step.
The high-pressure steam modifies the plant cell wall structure, yielding a dark brown material from which partially hydrolyzed hemicelluloses are easily recovered by water-washing, leaving a water-insoluble fraction composed of cellulose, residual hemicelluloses and a chemically modified lignin .
The band at 1514 cm-1 has been chosen as an internal standard, since this band is present in all spectra and it is well defined.
Relative intensity of bands in the infrared spectrum of different groups in the untreated and pretreated sugar cane bagasse samples
Assignment of FT-IR absorption of sugar cane bagasse
Relative absorbance of different groups in bagasse samples
Maximum band position (cm-1)
Pretreated bagasse with SO2
Pretreated bagasse with CO2
O-H stretching (H-bonded)
O-H vibration of phenolic group
O-H stretching of secondary alcohol
O-H stretching of primary alcohol
C-O stretching of phenols
C-H aliphatic axial deformation
C-H aliphatic angular deformation
C-H vibration of methoxyl group
C-H angular deformation of methoxyl group
C=C aromatic skeletal vibration
Relative absorbance of OCH 3 group (cm -1 ) according to the FTIR spectrum of the sugar cane bagasse
OCH3group bands (cm-1)
Pretreated bagasse with SO2
Pretreated bagasse with CO2
Relative absorbance of O-H group (cm -1 ) according to the FTIR spectrum of the sugar cane bagasse
OH group bands (cm-1)
Pretreated bagasse with SO2
Pretreated bagasse with CO2
Relative absorbance of aromatic ring (cm -1 ) according to the FTIR spectrum of the sugar cane bagasse
Aromatic ring bands (cm-1)
Pretreated bagasse with SO2
Pretreated bagasse with CO2
The absorption at 2920 cm-1 could be attributed to C-H aliphatic axial deformation in CH2 and CH3 groups from cellulose, lignin and hemicellulose.
Usually the absorptions of O-H stretching occur in 3100–3600 cm-1 range. The band observed at 3386 cm-1 seems to be characteristic of OH groups present in lignin and carbohydrates. From Table 3, it could be observed that this band has higher values of relative absorbance in the case of pretreated samples when compared to untreated one. This result could be attributed to the chemical changes observed when sugar cane bagasse is pretreated with SO2 or CO2.
The relative absorbance of the bands of primary and secondary OH groups at 1051 cm-1 and 1165 cm-1 of untreated sugar cane bagasse is lower than the pretreated ones (Tables 1 and 3). It is worth noting that the relative absorbance of pretreated bagasse with SO2 is even higher than the one pretreated with CO2. This could be explained by the fact that SO2 provides a lower pH and consequently a higher combined severity, which resulted in a more exposed structure.
According to Nada and co-workers , the band at 2852 cm-1 is assignable to vibration of OCH3 groups, which is commonly present in lignin (Table 2). This OCH3 group could also be attributed to acetyl from hemicellulose. It could be observed that only a slight increase of 6.5% and 5.5% of the relative absorbance of OCH3 groups after pretreatment using SO2 or CO2, respectively, as expected after an efficient pretreatment process.
When comparing the relative absorbance of the OCH3 group and OH group (Tables 2 and 3), it is possible to note that there was a significant increase in the relative absorbance after pretreatment of OH groups (31.9% and 28.8%, using SO2 and CO2 in the pretreatment, respectively), while this is not observed for the OCH3 groups (6.5% and 5.5%, using SO2 and CO2, respectively). This data indicate the conversion of lignin methoxyl groups into phenolic groups during pretreatment .
The bands at 1604 cm-1 and 1633 cm-1 are attributed to C-Ph and C=C, respectively. These bands are generally found in the lignin aromatic structure. The relative absorbance of these vibrations are higher (around 9.3%) after pretreatment (Table 4), which confirms the conversion of lignin methoxyl groups into phenolic groups.
The band at 1735 cm-1 is referred to the acetyl groups present in the hemicellulose. The pretreated bagasse with CO2 or SO2 exhibits a higher relative absorbance when compared to untreated sample 16.9% and 15.5%, respectively (Table 1). The former results can be explained by the amount of hemicelullose fraction removed in each pretreatment, 40.5% and 63.7% for using CO2 and SO2, respectively .
The signal at 897 cm-1 is attributed to β-glycosidic linkages between monosaccharide units and it is also higher for the pretreated samples (8.8% and 4.4% with SO2 and CO2, respectively), as expect after bagasse fibers exposure.
The analysis by SEM, TEM, XRD and FTIR spectroscopy of steam pretreated bagasse in the presence of CO2 at 205°C/15 min or SO2 at 190°C/5 min showed significant differences amongst the untreated and the pretreated materials. It was observed in the outer region of the cell wall (SCW), upon pretreatment, the formation of large pores with different sizes and shapes which were more prominent when SO2 was the impregnating agent. It was also observed in both cases the formation, in the cell wall, of coalescent particles with round or elongated shapes likely formed by lignin and/or hemicellulose.
The morphology of CO2-pretreated bagasse was more preserved than that of the SO2-preatrement, likely due to its lower combined severity factor of 0.9 in comparison to that of SO2− pretreatment of 1.7. It was also observed that both impregnating agents, SO2 or CO2, behaved in a quite similar way.
The crystallinity index values obtained from XRD patterns showed that pretreated materials have higher values (CI (SO2) = 65.5%, CI (CO2) = 56.4%) when compared with untreated material (CI = 42.5%), due to the partial removal from the bagasse of its hemicelluloses content. The results of FTIR spectra also showed changes in the chemical structure of materials pretreated with CO2 and SO2, mainly in OCH3, OH and C=O groups; which supported the data from the XRD, SEM and TEM analysis.
The use of SO2 and CO2 as an impregnating agent for sugar cane bagasse treatment was previously studied . In the present study the most promising pretreated materials were selected for further studies on structural modifications. Bagasse samples steam pretreated in the presence of CO2 (205°C/15 min) and SO2 (190°C/5 min) and also untreated bagasse were submitted to the following techniques: electron microscopy, X-ray diffraction and infrared spectroscopy. All samples were sieved (< 1.8 mm) before analyses.
Scanning electron microscopy (SEM)
Scanning electron microscopy (SEM - FEI / Inspect S50 model) was used to observe modifications on bagasse fibers. Samples were adhered to carbon tape and sputter coated with gold (sputter Emitech / K550 model) and observed in the SEM through the use of an acceleration voltage of 20 KV and working distance of around 38 mm. Hundreds of SEM images were obtained on different areas of the samples to guarantee the reproducibility of the results.
Transmission electron microscopy (TEM)
Transmission electron microscopy (FEI Tecnai G2 12 Spirit) was used to observe the ultrastructural changes within the cell wall. Each condition (untreated material, pretreated with SO2 and CO2 material) was analyzed in triplicate. Each individual sample was studied by an unbiased random selection of fibers that represent the total population. Samples were dehydrated in an increasing acetone series and embedded in Spurr resin. Ultrathin sections, 70nm, were obtained in the LEICA ultramicrotome and deposited onto copper grids. The sections were stained with 5% uranyl acetate and lead citrate and observed in the TEM with an acceleration voltage of 120 kV.
X-ray diffraction (XRD)
Where I002 is the intensity of plane 002 and Iam is related to the amorphous structure.
Infrared spectroscopy (FTIR)
The infrared spectra (wave numbers in cm-1) were obtained on a Magma - IR 560 E.S.P – Nicolet spectrophotometer, by means of a KBr disk containing 3% finely ground samples. Thirty-two scans were taken of each sample recorded from 4000 to 400 cm-1 at a resolution of 4 cm-1. The relative absorbance values were obtained with four decimal units; however, only two decimal units were plotted in the data showed in Tables 1, 2, 3 and 4.
Authors would like to thank the Brazilian Innovation Agency - (FINEP), the Ministry of Science, Technology and Innovation (MCTI) and the Brazilian Council for Research and Development (CNPq) for financial support. Authors are also thankful to Prof. Guido Zacchi and colleagues from the Chemical Engineering Department, Lund University. Authors would like to express their gratitude to colleagues from CENANO/INT/MCTI (Center of Nanostructure Characterization), especially to Sheyla Santana de Carvalho and Fernanda C.S.C. dos Santos.
- Mohanty AK, Misra M, Drzal LT: Sustainable biocomposites from renewable resources: Opportunities and challenges in the green materials world. J Polymer Environ 2002, 10:19–26.View Article
- Taherzadeh MJ, Karimi K: Enzymatic-based hydrolysis processes for ethanol from lignocellulosic materials: A review. Bioresource 2007, 2:707–738.
- UNICA: Brazilian Sugarcane Industry Association. http://www.unica.com.br/
- Pandey A, Soccol CR, Nigam P, Soccol VT: Biotechnological potential of agro-industrial residues. I. Sugarcane bagasse. Bioresour Technol 2000, 74:69–80.View Article
- Richardson S, Gorton L: Characterisation of the substituent distribution in starch and cellulose derivatives. Anal Chim Acta 2003, 497:27–65.View Article
- Fengel D, Wegener G: Wood: chemistry, ultrastructure, reactions. XII. Berlin, New York: Walter de Gruyter; 1989.
- Zhang YHP, Lynd LR: Toward an aggregated understanding of enzymatic hydrolysis of cellulose: Noncomplexed systems. Biotechnol Bioeng 2004, 88:797–824.View Article
- Yang B, Wyman CE: Pre-treatment: the key to unlocking low-cost cellulosic ethanol. Biofuels Bioprod Bioref 2008, 2:26–40.View Article
- Galbe M, Zacchi G: Pretreatment of Lignocellulosic Materials for Efficient Bioethanol Production. Adv Biochem Eng Biotechnol 2007, 108:41–67.
- Ferreira-Leitão V, Perrone CC, Rodrigues J, Franke APM, Macrelli S, Zacchi G: An approach to the utilisation of CO2as impregnating agent in steam pretreatement of sugar cane bagasse and leaves for ethanol production. Biotechonol Biofuels 2010, 3:1–8.View Article
- Perrone CC, Zacchi G: Processo para o pré-tratamento de biomassa lignocelulósica. Patent number (BR 0803354–4). Brazil; 2008.
- Rezende CA, Lima MA, Maziero P, Azevedo ER, Garcia W, Polikarpov I: Chemical and morphological characterization of sugarcane bagasse submitted to a delignification process for enhanced enzymatic digestibility. Biotechonol Biofuels 2011, 4:54.View Article
- Nada AAMA, El-Sakhawy M, Kamel SM: Infra-red spectroscopic study of lignins. Polymer Degrad Stability 1998, 60:247–251.View Article
- Rodrigues Filho G, De Assunção RMN, Vieira JG, Meireles CS, Cerqueira DA, Barud HS, Ribeiro SJL, Messaddeq Y: Characterization of methylcellulose produced from sugar cane bagasse cellulose: Crystallinity and thermal properties. Polymer Degrad Stability 2007, 92:205–210.View Article
- Chundawat SPS, Donohoe BS, Sousa LC, Elder T, Agarwal UP, Lu F, Ralph J, Himmel ME, Balan V, Dale BE: Multi-scale visualization and characterization of lignocellulosic plant cell wall deconstruction during thermochemical pretreatment. Energy Env Sci 2011, 4:973–984.View Article
- Grethlein HE: The effect of pore size distribution on the rate of enzymatic hydrolysis of cellulosic substrates. BioTechnol 1985, 3:155–160.View Article
- Donohoe BS, Selig MJ, Viamajala S, Vinzant TB, Adney WS, Himmel ME: Detecting cellulase penetration into corn stover cell walls by immuno-electron microscopy. Biotechnol Bioeng 2009, 103:480–489.View Article
- Chum H, Johnson DK, Black SK: Organosolv pretreatment for enzymic hydrolysis of poplars. 2. Catalyst effects and the combined severity parameter. Ind Eng Chem Res 1990, 29:156–162.View Article
- Tanahashi M, Takada S, Aoki GT, Higuchi T, Hanai S: Characterization of explosion Wood.1. Structure and physical properties. Wood Res 1983, 9:31–36.
- Ramos LP: The Chemistry involved in the steam treatment of lignocellulosic materials. Quim Nova 2003, 26:863–871.View Article
- Gastaldi G, Capretti G, Focher B, Cosentino C: Characterization and properties of cellulose isolated from the crambe abyssinica hull. Ind Crop Prod 1998, 8:205–218.View Article
- Li M-F, Yong-Ming F, Run-Cang S, Xu Feng: Characterization of extracted lignin of bamboo (Neosinocalamus affinis) pretreated with sodium Hydroxide/urea solution at low temperature. BioResour 2010, 5:1762–1778.
- Shao SL, Wen GF, Jin ZF: Changes in chemical characteristics of bamboo (Phyllostachys pubescens) components during steam explosion. Wood Sci Techonol 2008, 42:439–451.View Article
- Faix O: Classification of lignins from different botanical origins by FT-IR spectroscopy. Holzforschung 1991, 45:21–27.View Article
- Pretsch E, Clerc S, Simon R: Tables of Spectra Data for Structure Determination of Organic Compounds. 2nd edition. London: Springer-Verlag; 1989.
- Silverstein RM, Webster FX: Identificação Espectrométrica de Compostos Orgânicos. 6th edition. Brazil: LTC; 2000.
- Segal L, Creely JJ, Martin AE, Conrad CM: An Empirical Method for Estimating the Degree of Crystallinity of Native Cellulose Using the X-Ray Diffractometer. Text Res J 1959, 29:764–786.View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.